Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Survey

Document related concepts

no text concepts found

Transcript

Progress In Electromagnetics Research B, Vol. 7, 133–143, 2008 OMNI-DIRECTION REFLECTION IN ONE DIMENSIONAL PHOTONIC CRYSTAL R. Srivastava Department of Physics Udai Pratap Autonomous College Varanasi 221002, India K. B. Thapa Department of Physics U.I. E.T, C. S. J. M. University Kanpur-208024, India S. Pati Department of Physics Udai Pratap Autonomous College Varanasi 221002, India S. P. Ojha C. C. S. University Meerut 200005, India Abstract—It is well known that under certain conditions, one dimensional photonic crystal (1D-PC) displays total omni-directional reﬂection (ODR) band gaps. The enhancement of total omnidirectional reﬂection band gap in 1D-PC is calculated theoretically. Using Transfer Matrix Method (TMM) and Bloch theorem, the reﬂectivity of one dimensional periodic structure for TE and TM-modes at diﬀerent angles of incidence has been calculated. 134 Srivastava et al. 1. INTRODUCTION Over the past decades, much attention has been given to photonic crystals (PCs) as a new kind of optical materials [1–6]. These materials are based on the interaction between an optical ﬁeld and materials exhibiting periodicity on the scale of wave length. The main feature of photonic crystals is that they can prohibit the propagation of electromagnetic waves within a certain frequency range called photonic band gap (PBG). The materials containing PBG have many potential applications in optoelectronics and optical communication. For the optical range within which the main application is expected, most of experimental eﬀort has been concentrated on two dimensional and three dimensional photonic crystals. The application of two dimensional and three dimensional photonic crystals is limited. Complete two dimensional and three dimensional band gap can be realized in photonic crystals where the refractive index is periodically modulated in two- and three-dimension respectively [2, 6–10]. Besides two dimensional and three dimensional photonic crystals, the simplest periodic structure both in geometry and manipulating is a one dimensional stack of two types of layer which diﬀers in the dielectric constants. One dimensional photonic crystal is attractive since their production is more feasible at any wavelength scale and their analytical and numerical calculations are simpler. It has been shown that one dimensional photonic crystals can totally reﬂect arbitrary polarized, transverse-electric (TE) and transverse-magnetic (TM), lights i.e., omnidirectional reﬂection, at all angles within the PBGs, can take place even in the absence of a complete band gap i.e., these crystals exhibit the property of omni-directional reﬂection [4, 6, 11]. Recently, several research groups worldwide have reported that a simple-to-fabricate periodic one dimensional medium can have high reﬂectivity over a wide range of frequencies at all incident angles, i.e., an omnidirectional reﬂection. The total reﬂection band that occurs in any direction for TE and TM polarization is called omni-directional reﬂector mirror. One dimensional photonic crystal designed as Bragg mirror. Mirrors are of two basic varieties, a metallic mirror or omnidirectional reﬂector and a dielectric Bragg mirror. One dimensional photonic crystal is designed as Bragg mirror [12–20]. In particular, large parts of these one dimensional photonic crystals were designed for application in the infrared wavelength ranges. Several research groups have reported that a simpler to fabricate Bragg mirror suﬃces to design a low loss omni-directional reﬂector [21–29]. In 1998 Fink et al. [4] and Winn et al. [30] ﬁrst reported that the one dimensional dielectric lattice displays total omnidirection reﬂection Progress In Electromagnetics Research B, Vol. 7, 2008 135 for incident light under certain conditions. They constructed a stack of nine alternating micrometer thick layers of Polystyrene and Tellurium and demonstrated omnidirectional reﬂection over the wavelength range from 10 to 15 micrometers. Gallas et al. [31] reported the annealing eﬀect in the Si/SiO2 omni reﬂectors. Chen et al. [32] fabricated six bilayers of SiO2 and TiO2 quarter wave ﬁlms using the sol-gel method and found an omnidirectional PBG of about 70 nm in near IR range. Chigrin et al. [6, 18] fabricated a lattice consisting of 19 layers of Na3 AlF6 and ZnSe and found that omnidirectional photonic band gap exists in the spectral range 604.3–638.4 nm. Lee and Yao [33] studied a wide range of realistic fabrication parameters for the formation of omnidirectional photonic band gaps (PBGs) in one-dimensional photonic crystals, theoretically as well as experimentally. In this paper, the reﬂectivity of Na3 AlF6 /Ge multilayer structure has large values of total omni-directional reﬂection than experimentally observed. The thicknesses of the each layer are taken 50% of the total thickness of the unit cell for low and high index of refractions respectively. Such Na3 AlF6 /Ge multilayer structure has large total omni-directional reﬂection than experimentally observed values for same structure with 50% of total thickness of unit cell for each material. 2. THEORY The Helmholtz equation for considered periodic structure (photonic crystal); 2 + ω εr µr E =0 2E ∇ c2 (1) where ε(x)µ(x) = n2 (x), with n(x) is the refractive index. We deled with electromagnetic wave propagated in the x-direction and polarized linearly. We take the y-axis is the direction of the polarization. The electric ﬁeld of the propagated wave is denoted by the complex function E(x, y) for convenience E(x, y) = E(x)eiβy (2) √ where E(x) = Aj eikjx x + Bj e−ikjx x for nj = εj , β = ωc nj sin θ, ω kjx = c nj cos θj , θj is the angle of incidence, Aj , Bj are coeﬃcients of reﬂected and incidence wave respectively with j = 1, 2. The wave vectors of ﬁrst and second medium are k1x and k2x respectively. The can be obtained along y-axis; magnetic ﬁeld vector H ×E = i ∇ H ωµ (3) 136 Srivastava et al. Figure 1. Schematic of the multilayer system with the incident wave vector k, the electromagnetic mode convention E and B are the electric and magnetic ﬁelds, respectively. A periodic arrangement of a multilayer ﬁlm with refractive indices n1 and n2 and thickness d1 and d2 respectively is shown in Figure 1. This structure is surrounded by the refractive indices n0 and ns , called incidence and substrate medium. The solution for Equation (1) will be superposition of plane waves traveling to the right and to the left. Say, for layer with index n1 , the right going and left going plane waves have amplitudes A1 and B1 respectively and for layer with index n2 right going and left going planes waves have amplitudes C1 and D1 respectively. Hence for layer with index n1 the solution of Equation (2) is E(x) = A1 eik1x x + B1 e−ik1x x (4) E(x) = C1 eik2x (x−d1 ) + D1 e−ik2x (x−d1 ) (5) and for the layer with index n2 . The parameter k1x and k2x will be called the wave number, and the deﬁnition is given by k1x = ωc n1 cos θ1 and k2x = ωc n2 cos θ2 . At the interface between layers (x = d1 ), the Equations (2) and (3) are continuous. This gives a relation between plane waves amplitude; A1 C1 = M12 (6) D1 B1 Progress In Electromagnetics Research B, Vol. 7, 2008 with M12 1 2 1 + = 1 1− 2 k1x k2x k1x k2x ik1x d1 e ik1x d1 e 1 2 1 2 k1x 1− k2x k1x 1+ k2x −ik1x d1 137 e −ik1x d1 e (7) and also at x = d, the interface between layer with index n2 and n1 , continuity of the Equations (2) and (3) which gives; C1 A2 = M21 (8) B2 D1 where the matrix M21 is the same as (7) but with interchanging the indices. Using matrix Equations (7) and (8) and eliminating C1 and D1 , we found the matrix for binary structure; A2 A1 = M21 M12 (9a) B2 B1 or A2 B2 = Mi,j A1 B1 (9b) where Mi,j = M21 M 12 . The matrix of Mi,j is given element 1 1 by; M1,1 = cos(k2x d2 ) + 2 i γ + γ sin(k2x d2 ) , M1,2 = e−i k1x d1 + 12 i γ1 − γ sin(k2x d2 ) , M2,1 = M̄1,2 , M2,2 = M̄1,1 , with eik1x d1 γ= k1x k2x for TE-mode and γ = k1x ×n22 k2x ×n21 for TM-mode. For the period of the lattices, E(x, K) = UK (x)eiK(ω)x with UK (x) is a complex valued periodic function of the lattices UK (x) = UK (x + d). The thickness of the unit cell is given as d(= d1 + d2). The parameter K(ω) is called the Bloch wave number or Dispersion Relation. There is an explicit expression for K(ω) as follows; 1 1 K(ω) = cos−1 (10) T r [Mi,j ] d 2 with Mi,j given in Equation (9). So Equation (10) becomes; K(ω) = 1 cos−1 [cos (k1x d1 ) × cos (k2x d2 ) d 1 1 γ+ × sin (k1x d1 ) × sin (k2x d2 ) − 2 γ (11) 138 Srivastava et al. Considering the structure of N period of layers with alternately refractive indices n1 and n2 and thickness d1 and d2 , the coeﬃcients of propagating states in right and left side of the multilayer structures are calculated by multiplying transfer matrices of each cell. AN A0 = (Mi,j )1 × (Mi,j )2 × (Mi,j )3 . . . (Mi,j )N (12) B0 BN The reﬂectance coeﬃcient is given by, B0 rN = A0 BN =0 (13) The reﬂectance is obtained by taking absolute value of the reﬂectance coeﬃcient, R = (|rN |)2 (14) 3. RESULTS AND DISCUSSION For the sake of numerical calculation we take Na3 AlF6 /Ge dielectric material with low and high index contrast. The refractive index for Na3 AlF6 is n1 = 1.34 and for Ge is n2 = 4.2. Taking thickness of the each layer same a = b and d = a + b = 115 nm in the visible region. Applying transfer matrix method [34, 35] a graph is plotted between reﬂectance and wavelength. Figure 2 and Figure 3 shows the reﬂectivity of calculated spectra at diﬀerent angle 0◦ , 20◦ , 40◦ , 60◦ and 85◦ for TE and TM mode respectively and the ODR is found at 0◦ to 86◦ shown in Figure 4. Table 1. For Na3 AlF6 /Ge d = 115 nm and a = b). Angle (deg) TE (nm) Band width TM (nm) Band width 0 540–894 354 540–894 354 20 535–891 356 539–871 332 40 522–883 361 535–810 271 60 508–874 366 533–733 200 85 500–868 368 536–670 134 ODR range . . . . . . 540–670 nm and ODR width . . . . . . 130 nm It is clear from the Table that the transmission range for TE mode is 540–894 nm at normal incidence; at the angle of 20◦ the range is Progress In Electromagnetics Research B, Vol. 7, 2008 139 Figure 2. Transmittance curve Vs wavelength (nm) of Na3 AlF6 /Ge multilayer structure for TE mode at diﬀerent angle. Figure 3. Transmittance curve Vs wavelength (nm) of Na3 AlF6 /Ge multilayer structure for TM mode at diﬀerent angle. 535–891 nm; at the angle of 40◦ the range is 522–883 nm; at the angle of 60◦ the range is 508–874 nm; at the angle of 85◦ the range is 500– 868 nm. The transmission range for TM mode is 540–894 nm at normal incidence; at the angle of 20◦ the range is 539–871 nm; at the angle of 40◦ the range is 535–810 nm; at the angle of 60◦ the range is 533– 733 nm; at the angle of 85◦ the range is 536–670 nm.Hence the total omnidirection range for this multilayer structure is lies between 670– 540 nm and the width of the omnidirection range is very large 130 nm. 140 Srivastava et al. Figure 4. Omnidirectional gap of Na3 AlF6 /Ge multilayer structure for TE and TM mode at diﬀerent angle. 4. CONCLUSION In conclusion, we have shown theoretically that a one-dimensional dielectric structure can exhibit total omnidirectional reﬂection of incident light. Such a structure can be used as a very useful optical device in the optical industry. These ﬁndings should stimulate new experiments on controllable spontaneous emission of atoms, molecules and solid state micro-structures in the optical range [18]. REFERENCES 1. Yablonovitch, E., “Inhibited spontaneous emission in solid state physics and electronics,” Phys. Rev. Lett., Vol. 58, 2059–2062, 1987. Progress In Electromagnetics Research B, Vol. 7, 2008 141 2. Jonopoulos, J. D., P. Villeneuve, and S. Fan, “Photonic crystals: Putting a new twist on light,” Nature, Vol. 386 143–149, 1997. 3. Zheng, Q. R., Y. Q. Fu, and N. C. Yuan, “Characteristics of planar PBG structures with a cover layer,” Journal of Electromagnetic Waves and Applications, Vol. 20, 1439–1453, 2006. 4. Fink, Y., J. N. Winn, S. Fan, C. Chen, J. Michel, J. D. Joannopoulos, and E. L. Thomas, “A dielectric omnidirectional reﬂector,” Science, Vol. 282, 1679–1682, 1998. 5. Rojas, J. A. M., J. Alpuente, J. Piñeiro, and R. Sánchez, “Rigorous full vectorial analysis of electromagnetic wave propagation in 1D,” Progress In Electromagnetics Research, PIER 63, 89–105, 2006. 6. Chigrin, D. N., A. V. Lavrinenko, D. A. Yarotsky, and S. V. Gaponenko, “Observation of total omnidirectional reﬂection from a one-dimensional dielectric lattice,” Appl. Phys. A: Mater. Sci. Process., Vol. 68, 25–28, 1999. 7. Joannopoulos, J. D., R. D. Meade, and J. N. Winn, Photonic Crystals: Molding the Flow of Light, Princeton Univ. Press, Princeton, NJ, 1995. 8. Burstein, E. and C. Weisbuch, Conﬁned Electron and Photon: New Physics and Applications, Plenum Press, New York, 1995. 9. Soukoulis, C., Photonic Band Gap Materials, 71–91, Kluwer Academic, Dordrecht, 1996. 10. Knight, J. C., J. Broeng, T. A. Birks, and P. S. J. Russell, Science, Vol. 282, 1476, 1998. 11. Yablonovitch, E., “Photonic band-gap structures,” J. Opt. Soc. Amer. B, Vol. 10, 283–295, 1993. 12. Kurizki, G. and W. Hause, “Special issue on photonic crystals,” Journal of Modern Optics, Vol. 41, 171–172, 1994. 13. Deopura, M., C. K. Ullal, B. Temelkuran, and Y. Fink, “Dielectric omnidirectional visible reﬂector,” Optics Letters, Vol. 26, 1197– 1199, 2001. 14. Almeida, R. and Z. Wang, “Sol-gel preparation of one-dimensional photonic bandgap structures,” Proc. SPIE, Vol. 4655, 24–33, 2002. 15. Russell, P. S. J., S. Tredwell, and P. J. Roberts, “Full photonic bandgapes and spontaneous emission control in 1D multilayer dielectric structures,” Opt. Commun., Vol. 160, 66–71, 1999. 16. Guida, G., “Numerical studies of disordered photonic crystals,” Progress In Electromagnetics Research, PIER 41, 107–131, 2003. 17. Guenneu, S., A. Nicolet, F. Zolla, and S. Lasquellec, “Numerical and theoretical study of photonic crystal ﬁbers,” Progress In 142 Srivastava et al. Electromagnetics Research, PIER 41, 271–305, 2003. 18. Chigrin, D. N., A. V. Lavrinenko, D. A. Yarotsky, and S. V. Gaponenko, “All dielectric one dimensional periodic structures for total omnidirectional reﬂection and partial spontaneous emission control,” J. Lightwave Tech., Vol. 17, 2018– 2024, 1999. 19. Lekner, J., “Omnidirectional reﬂection by multilayer dielectric mirrors,” J. Opt. A: Pure Appl. Opt., Vol. 2, 349–352, 2000. 20. Zandi, O., Z. Atlasbaf, and K. Forooraghi, “Flat multilayer dielectric reﬂector antennas,” Progress In Electromagnetics Research, PIER 72, 1–19, 2007. 21. Dowling, J. P., “Mirror on the wall: You’re omnidirectional after all?” Science, Vol. 282, 1841–1843, 1998. 22. Yablonovitch, E., “Engineered omnidirectional externalreﬂectivity spectra from onedimensional layered interference ﬁlters,” Optics Letters, Vol. 23, 1648–1649, 1998. 23. Maka, T., D. N. Chigrin, S. G. Romanov, and C. M. Sotomayor Torres, “Three dimensional photonic crystals in the visible regime,” Progress In Electromagnetics Research, PIER 41, 307– 335, 2003. 24. Ozbay, E., B. Temelkuran, and M. Bayinder, “Microwave application of photonic crystals,” Progress In Electromagnetics Research, PIER 41, 185–209, 2003. 25. Aissaoui, M., J. Zaghdoudi, M. Kanzari, and B. Rezig, “Optical properties of the quasi-periodic one-dimensional generalized multilayer Fibonacci structures,” Progress In Electromagnetics Research, PIER 59, 69–83, 2006. 26. Zheng, Q. R., Y. Q. Fu, and N. C. Yuan, “Characteristics of planar PBG structures with a cover layer,” Journal of Electromagnetic Waves and Applications, Vol. 20, 1439–1453, 2006. 27. Srivastava, S. K. and S. P. Ojha, “Omnidirectional reﬂection bands in one-dimensional photonic crystals with left-handed materials,” Progress In Electromagnetics Research, PIER 68, 91– 111, 2007. 28. Srivastava, S. K. and S. P. Ojha, “Omnidirectional reﬂection bands in one-dimensional photonic crystal structure using ﬂuorescence ﬁlms,” Progress In Electromagnetics Research, PIER 74, 181–194, 2007. 29. Srivastava, R., S. Pati, and S. P. Ojha, “Enhancement of omnidirectional reﬂection in photonic crystal heterostructures,” Progress In Electromagnetics Research B, Vol. 1, 197–208, 2008. Progress In Electromagnetics Research B, Vol. 7, 2008 143 30. Winn, J. N., Y. Fink, S. Fan, and J. D. Joannopoulos, “Omnidirectional reﬂection from a one-dimensional photonic crystal,” Optics Letters, Vol. 23, 1573–1575, 1998. 31. Gallas, B., S. Fission, E. Charron, A. Brunet-Bruneau, R. Vuye, and J. Rivory, Appl. Opt., Vol. 40, 5056, 2001. 32. Chen, K. M., A. W. Sparks, H. C. Luan, D. R. Lim, K. Wada, and L. C. Kimerling, Appl. Phys. Lett., Vol. 75, 3805, 1999. 33. Lee, H.-Y. and T. Yao, “Design and evaluation of omnidirectional onedimensional photonic crystals,” J. Appl. Phys., Vol. 93, 819– 830, 2003. 34. Yeh, P., Optical Waves in Layered Media, John Wiley & Sons, New York, 1988. 35. Born, M. and E. Wolf, Principles of Optics, Cambridge University Press, Cambridge, 1998.

Related documents